RESISTANCE OF HARDWOODS TO CREOSOTE. 



21 



40r 

















































































































































_ 

















































'-'" 

















HICKORY 













































































































































































































































































































































































































































) 

















































. 

















































































































































































































































































































































































































































































































































































































































































































































■lEAr? 























_ 

















































G 

















































































































































4- 































































































































































































i 



















__ 

























i 



25 50 75 100 125 



PRESSURE- LBS. PER SQ. IW. 



4C 















J_ _ ±_L 





: 







































1 

























_, 















1 











36 











































$H!TE HEART BEECH 





















































32 









































































































































































f-28 

 o 



















































































o 











































"» 







































E24 

















































































U 











































e 



























































































































«-4*. 



a 

































J 



R* 







rhs 



_s 































/ 











+ -f 



S !E 

 o 





























/ 



































* 



, L 



7 











































fHSAl 



a 





























1 1 











S 

 <S 





























1 



































































































































1 



8 







< 







































> 







































[ 



( 











































i 







































4 



j 









































/ 









































/ 























I 

















1 























FOHEST PRODUCTS LfiSCR&TDSYl 





' 























a 



.1) 



5C 





ft 



9 





OCT., 1915] 



25 50 75 SOO i25 



PRESSURE- LBS. PER SQ. IM. 



Fig. 6. — Absorption in the heartwood of hickory and white-heart beech. 





l r- ' ■ — 



~r _ 







i_ 









± 









T^ 

















F.&U uUtn 









i 









































































































jfa».. Jr 





-j, 





>' "r|— — A h 







/ 









(^SA 



"WOOD 







s r 









J 









-/ 









I 









i4 









\t 



















































It 









i i 









It It.. 





-M 





HE* !»TWOO!J^>" 









~-<t-l— 1 A-n 







i e^" - 



Tttt- 







25 50 



FRESSURE- 



75 100 i£5 



i.S3. PER SQ. IN. 



















I 1 1 









































it IT 



































































s« 























1 































RED HEART BEECH 

























































































32 





































































































































































































&-28 



s 

































































































































































































£24 



































































































u 



















































K 



















































&20 



































































































a 



















































_i 



















































3 J6 





















































































































































3 

































































































































































J 



«, 

















































/ 





«J4EAI 



















8 





















N 



. 



























/ 























s 

























/ 





























> 





















/ 

































--. 













/ 









4 









































-Si 



', 























































































































- 











FOHEST PRODUCTS LABORArOR.r 









I 















a 



ill 



SI 



s<. 



* 



5. 











CT 



.li 



IS 



i 50 75 100 l?5 



PRESSURE-LBS. PER SO. i». 



Fig. 7. — Absorption in the heartwood of red gum and red-heart beech and the sapwood of 



red gum. 



